Energies 2020, 13, 537; doi:10.3390/en13030537 www.mdpi.com/journal/energies Article
Experimental Evidence of PID Effect on CIGS
Sofiane Boulhidja 1, Adel Mellit 1,2, Sebastian Voswinckel 3, Vanni Lughi 4, Alessandro Ciocia 5, Filippo Spertino 5 and Alessandro Massi Pavan 4,* 1 Renewable Energy Laboratory, Faculty of Sciences and Technology, Jijel University, Ouled‐Aissa P.O. Box. 98, Jijel 18000, Algeria; firstname.lastname@example.org (S.B.); email@example.com (A.M.) 2 The Abdus Salam International Centre for Theoretical Physics (ICTP), Strada Costiera, 11, 34151 Trieste, Italy 3 RET—Institute for Renewable Energy Technology, University of Applied Sciences Nordhausen Weinberghof 4, 99734 Nordhausen, Germany; voswinckel@fh‐nordhausen.de 4 Department of Engineering and Architecture, University of Trieste, Via A. Valerio, 6/A, 34127 Trieste, Italy; firstname.lastname@example.org 5 Department of Energy Engineering “Galileo Ferraris”, Polytechnic of Turin, Corso Duca Degli Abruzzi, 24, 10129 Turin, Italy; email@example.com (A.C.); firstname.lastname@example.org (F.S.) * Correspondence: email@example.com Received: 13 December 2019; Accepted: 20 January 2020; Published: 22 January 2020 Abstract: As well known, potential induced degradation (PID) strongly decreases the performance of photovoltaic (PV) strings made of several crystalline silicon modules in hot and wet climates. In this paper, PID tests have been performed on commercial copper indium gallium selenide (CIGS) modules to investigate if this degradation may be remarkable also for CIGS technology. The tests have been conducted inside an environmental chamber where the temperature has been set to 85 °C and the relative humidity to 85%. A negative potential of 1000 V has been applied to the PV modules in different configurations. The results demonstrate that there is a degradation affecting the maximum power point and the fill factor of the current‐voltage (I‐V) curves. In fact, the measurement of the I‐V curves at standard test condition show that all the parameters of the PV modules are influenced. This reveals that CIGS modules suffer PID under high negative voltage: this degradation occurs by different mechanisms, such as shunting, observed only in electroluminescence images of modules tested with negative bias. After the stress test, PID is partially recovered by applying a positive voltage of 1000 V and measuring the performance recovery of the degraded modules. The leakage currents flowing during the PID test in the chamber are measured with both positive and negative voltages; this analysis indicates a correlation between leakage current and power losses in case of negative potential. Keywords: photovoltaic modules; CIGS cells; bias; potential induced degradation; leakage current 1. Introduction
degradation (PID). PID occurs in both crystalline silicon and thin film PV modules and can considerably compromise the performance of a PV system, especially if this operates at a high DC voltage . PID can provoke catastrophic consequences in the operation of a PV system: in some cases, CIGS modules have essentially stopped functioning after bias application . Thus, it is important to understand how the PID phenomenon works and how to prevent it. The PID effect has received considerable attention; therefore, many researches were carried out on PID degradation occurring in crystalline silicon PV modules, which represent the most installed PV technology over the world. Hacke et al.  reported that a sample of polycrystalline silicon (p‐Si) modules inside an environmental chamber, with a temperature of 85 °C and a relative humidity of 85% under a negative voltage of 600 V, exhibited a decay of 80% in maximum power after a short time of the test. Nagel et al.  reported that, after maintaining p‐Si modules in the field under a negative voltage of 1000 V, they showed a power loss more than 50% within 25 weeks. Furthermore, Islam et al.  investigated the real PID of c‐Si modules installed in a power plant: they reported an on‐site power degradation of 46.5% after a duration of a negative voltage stress for nearly 11 years. Some authors reported a power loss range from 10% to 90% for various c‐Si modules (including mono and poly‐crystalline cells) after PID tests inside chamber . PID has been also tested on monocrystalline modules: Oh et al. reported that p‐base mono‐crystalline silicon cells lost approximately 50% of their initial power at −600 V after just 44 h . Goranti et al.  investigated that the remaining power of mono‐crystalline modules stressed at 85 °C dry heat, with negative voltage of 600 V was about 15% compared to the pre‐test power , as the c‐Si modules are affected by PID; some authors reported that coating a TiO2 thin film on the cover glass of modules can prevent them from PID . The PID in thin film modules is mostly attributed to the diffusion of Na+ ions originating from the module glasses, via different mechanisms depending on the presence or absence of moisture, and is often manifested through delamination or corrosion of the transparent conducting oxide (TCO) layer of the module. This can cause a drastic reduction of the module performance [10–13]; Fjällström et al.  reported that PID effect can drive the efficiency of CIGS cells to drop to about zero.
As well known, the PID effect highly depends on the environmental conditions, especially temperature and relative humidity. If a PV module is subject to high potential (with the proper sign) under these conditions, a drastic degradation of the module performance can happen: the degradation seems to be correlated with the leakage current flowing between the module frame, usually grounded, and the active parts of the solar cells; this current crosses the encapsulant material of the module. It has been reported that the leakage current flowing through the glass and the encapsulant leads to an accumulation of trapped negative charges on the active layer . There are different pathways for the leakage current to flow between the frame of the module and the solar cells. The pathway from the active layer to the frame through the front glass which has a high surface conductivity is the most dominant during the PID effect [16,17]. The low resistivity is mainly due to the encapsulant material: the soda‐lime glass used in thin‐film PV modules can be the source of sodium ions that, located at the front glass surface, might lead to a loss of the efficiency [18–20]. Even though the PID mechanism is not yet well understood, the sodium ions that migrate from the glass to the TCO seem to be one of the main reasons for the degradation . The migration of the sodium ions causes a cell shunting that leads to a reduction of the module efficiency together with a deterioration of the main electrical characteristics [14,21]. It has also been demonstrated that PID degraded modules can recover from their condition by applying a positive bias . The PID stress is related to the materials used to fabricate the modules and can be suppressed by using a sodium‐ free front cover glass, Yamaguchi et al. have reported that CIGS modules can be prevented from PID by using an ionomer encapsulant .
In this work, tests have been performed on some commercial CIGS modules working in an environmental chamber and connected to both a negative and a positive high voltage. The current voltage (I‐V) curves and the main electrical parameters have been collected and investigated. Electroluminescence imaging has been used in order to analyse the non‐visible degradation process. The leakage current flowing between the ground and the cells’ active layer has also been measured. A final “recovery” test has been performed in order to bring the PV modules back to their initial conditions. The adopted methodology and the results will be used as a reference for researchers that will compare them with new results obtained on CIGS modules from different manufacturers.
2. Diagnostics Techniques for PID Detection
The I‐V curve measurement and the electroluminescence (EL) test are two complementary diagnostics techniques. The I‐V curve measurement allows a quantitative evaluation of the PV module performance, while the EL gives a qualitative state of health, with details about the causes of the failures. 2.1. Description of Diagnostics Techniques for Defects Detection Regarding the determination of I‐V curves, the dynamic methods consist of the use of capacitive or electronic loads , with an adequate and calibrated measurement system . A typical scheme of the measurement system with capacitive load is shown in Figure 1; voltage, current, irradiance, and ambient temperature are detected simultaneously (the irradiance sensor and the thermometer for ambient temperature are not represented).
Figure 1. Measurement scheme for the I‐V characterization of a photovoltaic (PV) generator by capacitive load.
Thanks to the capacitive load , the scan of the entire I‐V curve can be easily performed at any level (module, string and array) up to hundreds of kilowatts. The elaboration of the I‐V curve points permits to obtain all the electrical parameters, in particular the actual power output and the performance of the module. The only limitation of the I‐V curve characterization is that it cannot easily provide information about the causes of the parameter deviations. In order to define the causes of underperformance, electroluminescence tests are even more used, thanks to higher accuracy and much lower costs than in the past .
The analysis of the EL images permits to justify the performance deviation with mechanical/chemical defects. The EL test starts with a forward bias of the PV module, obtained thanks to an appropriate DC power supply (Figure 2), in a totally shaded condition (e.g., in a dark room of a laboratory or on‐field with low irradiance). The PV cells work like light emitting diodes (LEDs), in which their semiconductor materials have emission spectra in the infrared (IR) region of PV generator
Hall effect probe
the electromagnetic spectrum and not in the visible region . The image, captured by the sensor, is post processed to permit the identification of the defects.
Figure 2. Scheme for the electroluminescence (EL) test of a PV module.
In case of c‐Si silicon modules, the IR emission is in the range 900–1300 nm, and the peak, corresponding to the bandgap, is at 1150 nm. This emission can be partially detected by cheap silicon sensors, i.e., silicon charge‐coupled device (CCD) or CMOS. On the other hand, the use of an expensive sensitive camera equipped with indium gallium arsenide (InGaAs) photodiodes is necessary for CIGS . In case of CIGS generators, the emission curve can reach a wavelength of 1400 nm and it is better matched by the absorption curve of an InGaAs detector.
2.2. Detection of PID
in an intermediate situation, in which they are partially working. In order to make a comparison between PID and other defects, the module shown in Figure 3 is affected by both PID and cracks. Actually, this figure refers to modules installed on a rooftop, and cracks appear due to the walking on the PV modules mainly during maintenance . The cracked cell is highlighted by a blue circle in Figure 3; the crack is easily identifiable because the black/inactive area has well‐defined edges. Another aspect which supports in the identification of PID is the distribution of inactive cells along the PV strings. As well described in the next chapter, the PID occurs when a high negative voltage is applied between the cells (n‐type layer in contact with the glass) and the metallic frame. Thus, supposing a floating voltage of the PV generator (in case of transformerless DC/AC converters), the most affected modules will be the ones at the end of the string (near the negative pole of the string), where there is a negative potential with respect to the ground (Figure 4). (a) (b) Figure 4. (a) EL image of a PV string of c‐Si cells affected by PID; (b) identification of modules affected by a negative potential between the PV cells and the metallic frame connected to ground. 3. Experimental Setup Degradation Figure 5 represents the sketch of the PID test in the climatic chamber. In the present work, a commercial device made by ATT Angelantoni Test technologies is used. It has a test volume of 11 m³, the temperature range is from −60 to +100 °C and the relative humidity can be controlled between 10% and 95%. The tests have been performed in three different configurations, as follows. In the first configuration, the positive terminal of the DC power supply has been connected to the front surface of the PV modules (a metallic foil is placed on the surface to equalize the electric potential), while the negative terminal with high voltage of 1000 V has been connected to the PV terminals in short circuit. In the second one, the only difference is that the positive terminal of the DC power supply has been connected to the back surface (by the same metallic foil). In the third one, the positive terminal of the DC power supply has been connected to the frame of the PV modules. The CIGS modules under study are four. the p‐type (CIGS) is rear‐side and n‐type (CdS) is front‐side. The frames of three modules, subject to artificial PID, have been grounded and one module without bias has been used as a reference, remaining at beginning of life.
Figure 5. PID setup with grounded frame, the PV connectors are shorted and connected to the
negative potential of the power supply.
The specifications of these PV modules (Bosch Solar) at STC are: maximum power Pmax = 74.6 W,
open circuit voltage Voc = 71.7 V, short circuit current Isc = 1.47 A, voltage at maximum power point
Vmpp = 56.5 V, and current at maximum power point Impp = 1.32 A. The power tolerance is ±5%. Firstly, the PV modules have been placed in an environmental chamber, where the temperature has been maintained at a constant value of 85 °C, and the relative humidity has been set to 85%. After the desired conditions have been reached, a negative voltage bias (1000 V) has been applied to the shorted leads of the modules, while their frames have been grounded. After a first cycle of about 20 h, the modules have been removed from the chamber and characterized using a flash tester, recording the I‐V curves as well as calculating the electrical parameters (including short circuit current Isc and Voc). The flash tests have been performed at the standard test conditions (STC): irradiance of 1000
W/m2, corresponding to air mass 1.5, and cell temperature of 25 °C. STC conditions have been
obtained in a dark room with temperature control and an artificial light. A pulsed solar simulator (PSS 8 from Berger) has been used; it consists of a Xenon flash tube; resistive loads are used to trace the I‐V curves. According to IEC 60904‐9 , the simulated spectrum AM 1.5 G, the spatial
uniformity and the temporal stability outperform A class . The measurements are acquired by a data acquisition system (12 bit‐resolution) with typical uncertainty <0.5% for both voltage and current and 1% for power. Afterwards, the modules have been placed again in the chamber to continue the PID test. The flash test measurements have been frequently repeated after about 20 h until the end of the test with a total duration of 120 h.
tester. Furthermore, the leakage current has been logged continuously for all the modules and the EL images have been taken before and after the tests inside the chamber. 4. Results and Discussion 4.1. Degradation All the modules have been characterised at STC conditions. Figure 6 shows the I‐V curves of three modules tested inside the climatic chamber with both negative (front contact of the first test) and positive (front contact of the second test) bias of 1000 V, and an unbiased module used as a reference. As shown in Figure 6, both the positive biased module and the unbiased module show similar behaviour with slight degradation, mainly due to the expected effect of high temperature and relative humidity inside the environmental chamber. On the contrary, the negative bias drives the sample to degrade significantly at the end of the test compared to the other samples. These results reveal that the high negative voltage induces PID degradation, in the CIGS modules under tests, with a remarkable power loss similar to the power losses in the crystalline silicon modules from different manufacturers. It is worth noting that the PID affected modules have not shown any visible discoloration.
The changes in electrical parameters of the modules during the tests with positive bias have been investigated: these changes result linked with the applied bias and environmental conditions inside the climatic chamber. Figure 7 shows the normalized values (with respect to the initial values) of the maximum power, Pmax, and the Fill Factor FF = Pmax/(Isc ∙Voc) as a function of stress time inside the
climatic chamber. Here, the connections are different: positive bias (1000 V) applied to the front contact, to the back contact, to the frame, and unbiased module.
Figure 6. I‐V curves of the three modules before (solid lines) and after (dotted lines) the tests in
Figure 7. Normalized maximum power (solid lines) and fill factor (dashed lines) of the tested modules
as a function of time with positive voltage.
Before the PID tests, for all the modules (four) the measured maximum powers have been very similar (Pmax,r = 77 W) and the corresponding fill factor has been FFr = 68%, where the deviations are
smaller than the uncertainty of the data acquisition system (±0.5% for both voltage and current, ±1% for power). In order to easily show the deviations, normalized values are used: they are calculated as the ratio between the measured value after the test and the initial value. In the first hours inside the
chamber, all the modules have exhibited a noticeable degradation of Pmax and FF. Normalized Pmax
has been reduced: the back contact and unbiased modules have rapidly highlighted a similar behaviour and decreased slowly down to 0.92 and 0.93 respectively, while the front and frame contacts have been degraded to 0.95 at the end of the test. Fill factor has shown a decrease to 0.98 with a similar behaviour for the front and frame contacts, while the FF for the back contact and unbiased modules has been degraded to 0.95. These results reveal that testing under harsh enviromental conditions and high voltage can have a slight effect on the modules performance, the damp‐heat conditions(85 °C/85% RH) lead to losses in the FF of CIGS cells. The decrease of the FF can be associated with an increase of series resistance, that is mainly caused by an enhancement in the resistivity of the transparent conductive oxide (TCO) layers. In [32,33], it is confirmed that this is the cause of performance losses of PV modules in damp‐heat conditions. The PV modules with front and frame contact connections have shown less degradation, because the forward bias has maintained the PV modules at a stable condition; on the contrary, the unbiased module has shown an higher performance degradation . Taking into account the measurement uncertainties (typical amount of ±1% for the current and the voltage values) arising during the flash testing, the evolution of the parameters can be attributed to metastabilities changes. Figure 8 shows the time evolution of the normalized parameters of the five modules under test with negative voltage of 1000 V. The results demonstrate that the PID effect is similar in the case of the tests with the back and the front contacts. After 120 h, even if Voc and Isc have remained constant,
both the maximum power and the fill factor have substantially decreased with the stress time. Really,
as shown in Figure 8, the average of Pmax and FF has been decreased by 35% at the end of the test.
These degradations lead to a significant reduction in the efficiency of the modules and in their capability to produce energy. In the case of light soaked modules, Pmax and FF have decreased
Figure 8. Parameters of the modules with different contacts as a function of time. The dotted lines
refer to the light soaked modules.
The exposure to 120 h of stress in the chamber has caused an increase of ≈12% of Voc in the
modules with both front and back contacts, respectively. On the contrary, the frame contact module
has decreased only by 3%. The Isc exhibits slight degradation, it has dropped by 3% and 6% for the
front and back contact tests, respectively. The degradation can be affected also by other parameters, however, the data reveal that the degradation of the modules is associated to a large decrease in the shunt resistance Rp (about 80%) and to an even more dramatic increase of the series resistance Rs (by
a factor of about 7), which affect the fill factor. It is evident that all electrical parameters of the frame contact module seem to be slightly changed after the PID test. It is worth noting that the evolution of the electrical parameters is only marginally influenced by the preliminary light soaking. Conversely, a small increase of the fill factor and of the short circuit current is observed during the first hours. This is due to the metastabilities of the PV modules in CIGS [35,36] and does not prevent the degradation of the modules because of the strong PID effect. Another important indication is that the positive bias does not influence much the performance of the modules, while the negative bias leads to an extensive degradation of their performance
parameters, while the PV modules have not shown any visible degradation nor any corrosion in the TCO layer. The EL images remarkably prove wide darkening areas, this consideration is applied to the front contact (Figure 9a) as well as for the back contact (Figure 9b), where a huge darkening area can be observed in the middle of the module, which is corresponding to the shunt resistance degradation highlighted in Figure 8, while the test with the frame shows a small degradation around the perimeter. Obviously, there are no changes in the EL images of the fourth module (Figure 9d) that was not stressed and has been kept new as a reference module. On the other hand, in case of crystalline silicon modules affected by PID, the inactive cells belong to the modules subject to a more negative potential (close to the negative pole of the PV string) and are located along the borders near the frame. (a) (b) (c) (d)
Figure 9. EL images of the tested modules at 85 °C and 85% RH, before (upper images) and after
(lower images) the test for different contacts: (a) front, (b) back, (c) frame, and (d) unbiased.
The dark regions shown in the EL images, which are due to the shunting mechanisms occurring in the middle or near the edge of the modules because of the contact used to apply the voltage for the PID test. Therefore, for both front and back contacts, the current is concentrating in the middle of modules, whereas for frame contact the current is concentrating at the edge and affects less the module. This witnesses the extensive degradation of the modules together with the big changes observed for the electrical parameters.
zone. This phenomenon, which might be the cause of the shunt resistance drop, certainly reduces the open circuit voltage and the short circuit current with a consequent loss of power.
On the other hand, the dark areas shown in the EL images are also related to the obvious increase of the series resistance shown in Figure 8, the luminescence emission is variable due to the sheet resistance of the TCO and the Mo back layer . The dark areas represent parts of a module where there is a poor or even a zero current flow. The increased value of the series resistance is the cause of the degradation of the fill factor.
As shown in the previous section, the critical environmental conditions together with the application of a high negative bias lead to a significant degradation of the main parameters of the modules and to a consistent efficiency loss. As the negative bias has been recognized to be the main cause of the degradation occurred during the test, a second test has been performed in order to show how an opposite bias could contribute to recover the modules.
Table 1 shows the changes in the electrical parameters of the degraded modules (front, back, and frame contacts) after the first PID test. The PV modules have been placed in the environmental chamber at a temperature of 85 °C and a relative humidity of 85%; a positive voltage of 1000 V has been applied for 120 h.
Table 1. Normalized electrical parameters to pre‐PID test value of modules, before and after the
Parameter After the PID Test (Before Recovery) After the Recovery Test
Back Front Frame Back Front Frame
Pmax [%] 0.55 0.56 0.91 0.64 0.75 0.89
FF [%] 0.66 0.64 0.92 0.68 0.75 0.92
Isc [%] 0.93 0.96 1.00 0.97 0.99 1.00
Voc [%] 0.89 0.87 0.97 0.96 0.96 0.96
(a) (b) (c) Figure 10. Electroluminescence images of the PV modules after the recovery test: (a) back contact, (b) front contact, and (c) frame contact. 4.3. Leakage Current Analysis A third analysis has been carried out on the leakage current flowing during the PID test (voltage 1000 V, temperature 85 °C, relative humidity 85%) which increases the surface conductivity of the modules. The leakage currents known as the transferred charges from the active layer to the frame, are plotted in Figure 11; these leakage currents are related to the PID effect. The highest current has been observed for the front contact configuration and corresponds to high degradation as displayed in Figure 8. Furthermore, the back contact module shows less flow: as both front and back connections cause significant degradations, this reveals that the leakage current through the back contact is most harmful than the front contact, and the power loss needs less transferred charges . The frame contact module shows the smallest leakage current which is related to a small degradation in the first test. These results could give a correlation between power loss and the leakage current flowing under high voltage during PID test.
Figure 11. Leakage currents in three conditions under negative voltage: rear side, front side, and
of soda‐lime glass in PV modules’ technologies leads that sodium ions located at the front glass surface decrease their resistivity, and drive to significant leakage current to flow through this path. It is considered as a dominant path of leakage current, when a high voltage is applied. On the other hand, the back surface has more resistivity compared to the front glass explained by the small amount of Na. This can reveal for less leakage current to flow as obtained after measurements. The obtained results after the PID test can be correlated with the magnitude of leakage current generated by bias in damp‐heat conditions, and flowing between the ground and the active cells: it reveals that the more the PID degradation occurs on PV modules, the more leakage current to flow in the modules. This correlation can be considered as an indicator of PID effect on PV modules. Figure 12 depicts the results of leakage current flowing in the three modules after applying the positive bias. However, the analysis of leakage current during recovery process shows that similar magnitude of current to flow in the opposite direction, as during PID stress, where the leakage current flowing through the front side has decreased more than a half at the end of the test.
Figure 12. Leakage current progress during tests with high positive voltage of 1000 V.
bias to the front side has been driven to partially recover the degraded performance of PID affected modules.
15. Hacke, P.; Smith, R.; Terwilliger, K.; Glick, S.; Pankow, J.; Kloss, M.; Kurtz, S. System voltage potential‐ induced degradation mechanisms in PV modules and methods for test. In Proceedings of the 2011 37th IEEE Photovoltaic Specialists Conference (PVSC), Seattle, WA, USA, 19–24 June 2011. 16. Voswinckel, S.; Wesselak, V.; Fokuhl, E.; Schmidt, C.; Watzlawik, K. Dos and don’ts of leakage current measurement. In Proceedings of the 31th European Solar Energy Conference and Exhibition, Hamburg, Germany, 14–18 September 2015. 17. Manz, P.; Wesselak, V.; Voswinckel, S.; Trautmann, B.; Fokuhl, E.; Schmidt, C. Leakage current pathways and magnitudes in correlation to PID of CIGS thin film modules. In Proceedings of the 29th European Solar Energy Conference and Exhibition, Amsterdam, Netherlands, 22–26 September 2014. 18. Colli, A. The role of sodium in photovoltaic devices under high voltage stress: A holistic approach to understand unsolved aspects. Renew. Energy 2013, 60, 162–168.
19. Schroeder, D.J.; Rockett, A.A. Electronic effects of sodium in epitaxial CuIn1−x Gax Se2. J. Appl. Phys. 1997,